#------------------------------------------------------------------------------
#$Date: 2016-03-23 01:56:35 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179162 $
#$URL: svn://www.crystallography.net/cod/cif/4/31/23/4312301.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4312301
loop_
_publ_author_name
'X. Z. Li'
'C. Wang'
'X. L. Chen'
'H. Li'
'L. S. Jia'
'L. Wu'
'Y. X. Du'
'Y. P. Xu'
_publ_section_title
;
 Syntheses, Thermal Stability, and Structure Determination of the Novel
 Isostructural RBa3B9O18 (R = Y, Pr, Nd, Sm, Eu, Gd, Tb, Dy, Ho, Er, Tm,
 Yb)
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              8555
_journal_page_last               8560
_journal_paper_doi               10.1021/ic049710m
_journal_volume                  43
_journal_year                    2004
_chemical_formula_sum            'B9 Ba3 O18 Y'
_chemical_formula_weight         886.22
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   7.1761(6)
_cell_length_b                   7.1761(6)
_cell_length_c                   16.966(2)
_cell_measurement_reflns_used    7192
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      33.5
_cell_measurement_theta_min      3.3
_cell_volume                     756.64(13)
_computing_cell_refinement       'Bruker XSCANS(Bruker,1997)'
_computing_data_collection       'Bruker XSCANS(Bruker,1997)'
_computing_data_reduction        'Bruker XSCANS(Bruker,1997)'
_computing_molecular_graphics    'BALLS & STICKS(Kang & Ozawa, 2002)'
_computing_publication_material  'Bruker SHELXL97(Sheldrick, 1997)'
_computing_structure_refinement  'Bruker SHELXL97(Sheldrick, 1997)'
_computing_structure_solution    'Bruker SHELXL97(Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 15\\times15microns
_diffrn_measured_fraction_theta_full 0.967
_diffrn_measured_fraction_theta_max 0.967
_diffrn_measurement_device_type  'Bruker Smart APEX-CCD'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0450
_diffrn_reflns_av_sigmaI/netI    0.0290
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            7174
_diffrn_reflns_theta_full        33.57
_diffrn_reflns_theta_max         33.57
_diffrn_reflns_theta_min         2.40
_exptl_absorpt_coefficient_mu    11.601
_exptl_absorpt_correction_T_max  0.560
_exptl_absorpt_correction_T_min  0.341
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   '(SADABS; Sheldrick, 1996)'
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    3.889
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    .
_exptl_crystal_description       block
_exptl_crystal_F_000             792
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.05
_refine_diff_density_max         10.015
_refine_diff_density_min         -11.041
_refine_diff_density_rms         0.448
_refine_ls_extinction_coef       0.0013(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.169
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     54
_refine_ls_number_reflns         1006
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.169
_refine_ls_R_factor_all          0.0568
_refine_ls_R_factor_gt           0.0513
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0337P)²+22.6787P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1297
_refine_ls_wR_factor_ref         0.1328
_reflns_number_gt                884
_reflns_number_total             1006
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic049710msi20040620_033910.cif
_cod_data_source_block           ybbo91
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Hexagonal' changed to 'hexagonal'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_cell_volume        756.62(13)
_cod_database_code               4312301
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'x-y, x, z+1/2'
'-y, x-y, z'
'-x, -y, z+1/2'
'-x+y, -x, z'
'y, -x+y, z+1/2'
'-x, -y, -z'
'-x+y, -x, -z-1/2'
'y, -x+y, -z'
'x, y, -z-1/2'
'x-y, x, -z'
'-y, x-y, -z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ba1 Ba 0.6667 0.3333 0.13111(4) 0.0120(2) Uani 1 3 d S . .
Y1 Y 0.0000 0.0000 0.0000 0.0101(3) Uani 1 6 d S . .
Ba2 Ba 0.0000 0.0000 0.2500 0.0522(6) Uani 1 6 d S . .
O1 O 0.2916(12) -0.1660(11) 0.2500 0.0146(13) Uani 1 2 d S . .
O2 O 0.4977(8) -0.1226(8) 0.0811(4) 0.0166(9) Uani 1 1 d . . .
O3 O 0.6692(11) 0.0815(11) 0.2500 0.0132(12) Uani 1 2 d S . .
B1 B 0.5065(18) -0.1145(18) 0.2500 0.0122(17) Uani 1 2 d S . .
O4 O -0.2485(8) -0.2461(8) 0.0818(3) 0.0152(9) Uani 1 1 d . . .
B2 B -0.4488(12) -0.2854(12) 0.0827(4) 0.0121(12) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Y Y -2.7962 3.5667 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3 Ba1 O3 70.85(17) 8_666 . ?
O3 Ba1 O3 70.85(17) 8_666 3_655 ?
O3 Ba1 O3 70.85(17) . 3_655 ?
O3 Ba1 O4 77.94(17) 8_666 3 ?
O3 Ba1 O4 90.69(18) . 3 ?
O3 Ba1 O4 147.47(16) 3_655 3 ?
O3 Ba1 O4 90.69(18) 8_666 1_665 ?
O3 Ba1 O4 147.47(16) . 1_665 ?
O3 Ba1 O4 77.94(17) 3_655 1_665 ?
O4 Ba1 O4 111.96(10) 3 1_665 ?
O3 Ba1 O4 147.47(16) 8_666 5_655 ?
O3 Ba1 O4 77.94(17) . 5_655 ?
O3 Ba1 O4 90.69(18) 3_655 5_655 ?
O4 Ba1 O4 111.96(10) 3 5_655 ?
O4 Ba1 O4 111.96(10) 1_665 5_655 ?
O3 Ba1 O2 67.40(16) 8_666 5_665 ?
O3 Ba1 O2 135.77(18) . 5_665 ?
O3 Ba1 O2 107.47(18) 3_655 5_665 ?
O4 Ba1 O2 67.13(14) 3 5_665 ?
O4 Ba1 O2 47.29(14) 1_665 5_665 ?
O4 Ba1 O2 145.10(15) 5_655 5_665 ?
O3 Ba1 O2 135.77(18) 8_666 3_655 ?
O3 Ba1 O2 107.47(18) . 3_655 ?
O3 Ba1 O2 67.40(16) 3_655 3_655 ?
O4 Ba1 O2 145.09(15) 3 3_655 ?
O4 Ba1 O2 67.13(14) 1_665 3_655 ?
O4 Ba1 O2 47.29(14) 5_655 3_655 ?
O2 Ba1 O2 112.29(10) 5_665 3_655 ?
O3 Ba1 O2 107.47(18) 8_666 . ?
O3 Ba1 O2 67.40(16) . . ?
O3 Ba1 O2 135.77(18) 3_655 . ?
O4 Ba1 O2 47.29(14) 3 . ?
O4 Ba1 O2 145.09(15) 1_665 . ?
O4 Ba1 O2 67.13(14) 5_655 . ?
O2 Ba1 O2 112.29(10) 5_665 . ?
O2 Ba1 O2 112.29(10) 3_655 . ?
O3 Ba1 B2 75.30(18) 8_666 1_665 ?
O3 Ba1 B2 144.76(17) . 1_665 ?
O3 Ba1 B2 89.2(2) 3_655 1_665 ?
O4 Ba1 B2 91.62(16) 3 1_665 ?
O4 Ba1 B2 23.09(15) 1_665 1_665 ?
O4 Ba1 B2 132.64(16) 5_655 1_665 ?
O2 Ba1 B2 24.84(16) 5_665 1_665 ?
O2 Ba1 B2 90.01(16) 3_655 1_665 ?
O2 Ba1 B2 134.23(16) . 1_665 ?
O3 Ba1 B2 89.2(2) 8_666 3 ?
O3 Ba1 B2 75.30(18) . 3 ?
O3 Ba1 B2 144.76(17) 3_655 3 ?
O4 Ba1 B2 23.08(15) 3 3 ?
O4 Ba1 B2 132.64(16) 1_665 3 ?
O4 Ba1 B2 91.62(16) 5_655 3 ?
O2 Ba1 B2 90.01(16) 5_665 3 ?
O2 Ba1 B2 134.23(16) 3_655 3 ?
O2 Ba1 B2 24.83(16) . 3 ?
B2 Ba1 B2 114.14(10) 1_665 3 ?
O3 Ba1 B2 144.76(17) 8_666 5_655 ?
O3 Ba1 B2 89.2(2) . 5_655 ?
O3 Ba1 B2 75.30(18) 3_655 5_655 ?
O4 Ba1 B2 132.64(16) 3 5_655 ?
O4 Ba1 B2 91.62(16) 1_665 5_655 ?
O4 Ba1 B2 23.08(15) 5_655 5_655 ?
O2 Ba1 B2 134.23(16) 5_665 5_655 ?
O2 Ba1 B2 24.84(16) 3_655 5_655 ?
O2 Ba1 B2 90.01(16) . 5_655 ?
B2 Ba1 B2 114.14(10) 1_665 5_655 ?
B2 Ba1 B2 114.14(10) 3 5_655 ?
O4 Y1 O4 93.9(2) 9 5 ?
O4 Y1 O4 86.1(2) 9 11 ?
O4 Y1 O4 179.999(1) 5 11 ?
O4 Y1 O4 86.1(2) 9 7 ?
O4 Y1 O4 93.9(2) 5 7 ?
O4 Y1 O4 86.1(2) 11 7 ?
O4 Y1 O4 180.0 9 3 ?
O4 Y1 O4 86.1(2) 5 3 ?
O4 Y1 O4 93.9(2) 11 3 ?
O4 Y1 O4 93.9(2) 7 3 ?
O4 Y1 O4 93.9(2) 9 . ?
O4 Y1 O4 86.1(2) 5 . ?
O4 Y1 O4 93.9(2) 11 . ?
O4 Y1 O4 180.0 7 . ?
O4 Y1 O4 86.1(2) 3 . ?
O4 Y1 Ba2 51.99(14) 9 7 ?
O4 Y1 Ba2 128.01(14) 5 7 ?
O4 Y1 Ba2 51.99(14) 11 7 ?
O4 Y1 Ba2 51.99(14) 7 7 ?
O4 Y1 Ba2 128.01(14) 3 7 ?
O4 Y1 Ba2 128.01(14) . 7 ?
O4 Y1 Ba2 128.01(14) 9 . ?
O4 Y1 Ba2 51.99(14) 5 . ?
O4 Y1 Ba2 128.01(14) 11 . ?
O4 Y1 Ba2 128.01(14) 7 . ?
O4 Y1 Ba2 51.99(14) 3 . ?
O4 Y1 Ba2 51.99(14) . . ?
Ba2 Y1 Ba2 180.0 7 . ?
O3 Ba2 O3 120.001(1) 1_455 3_545 ?
O3 Ba2 O3 120.000(1) 1_455 8_666 ?
O3 Ba2 O3 120.0 3_545 8_666 ?
O3 Ba2 O1 49.8(2) 1_455 8_556 ?
O3 Ba2 O1 70.2(2) 3_545 8_556 ?
O3 Ba2 O1 169.8(2) 8_666 8_556 ?
O3 Ba2 O1 169.8(2) 1_455 . ?
O3 Ba2 O1 49.8(2) 3_545 . ?
O3 Ba2 O1 70.2(2) 8_666 . ?
O1 Ba2 O1 120.000(1) 8_556 . ?
O3 Ba2 O1 70.2(2) 1_455 3 ?
O3 Ba2 O1 169.8(2) 3_545 3 ?
O3 Ba2 O1 49.8(2) 8_666 3 ?
O1 Ba2 O1 120.001(1) 8_556 3 ?
O1 Ba2 O1 119.999(1) . 3 ?
O3 Ba2 B1 23.6(2) 1_455 1_455 ?
O3 Ba2 B1 96.4(2) 3_545 1_455 ?
O3 Ba2 B1 143.6(2) 8_666 1_455 ?
O1 Ba2 B1 26.2(2) 8_556 1_455 ?
O1 Ba2 B1 146.2(2) . 1_455 ?
O1 Ba2 B1 93.8(2) 3 1_455 ?
O3 Ba2 B1 96.4(2) 1_455 8_666 ?
O3 Ba2 B1 143.6(2) 3_545 8_666 ?
O3 Ba2 B1 23.6(2) 8_666 8_666 ?
O1 Ba2 B1 146.2(2) 8_556 8_666 ?
O1 Ba2 B1 93.8(2) . 8_666 ?
O1 Ba2 B1 26.2(2) 3 8_666 ?
B1 Ba2 B1 120.0 1_455 8_666 ?
O3 Ba2 B1 143.6(2) 1_455 3_545 ?
O3 Ba2 B1 23.6(2) 3_545 3_545 ?
O3 Ba2 B1 96.4(2) 8_666 3_545 ?
O1 Ba2 B1 93.8(2) 8_556 3_545 ?
O1 Ba2 B1 26.2(2) . 3_545 ?
O1 Ba2 B1 146.2(2) 3 3_545 ?
B1 Ba2 B1 120.000(2) 1_455 3_545 ?
B1 Ba2 B1 119.999(2) 8_666 3_545 ?
O3 Ba2 Y1 90.0 1_455 2 ?
O3 Ba2 Y1 90.000(1) 3_545 2 ?
O3 Ba2 Y1 90.000(1) 8_666 2 ?
O1 Ba2 Y1 90.0 8_556 2 ?
O1 Ba2 Y1 90.0 . 2 ?
O1 Ba2 Y1 90.0 3 2 ?
B1 Ba2 Y1 90.000(1) 1_455 2 ?
B1 Ba2 Y1 90.000(1) 8_666 2 ?
B1 Ba2 Y1 90.000(1) 3_545 2 ?
O3 Ba2 Y1 90.0 1_455 . ?
O3 Ba2 Y1 90.0 3_545 . ?
O3 Ba2 Y1 90.0 8_666 . ?
O1 Ba2 Y1 90.0 8_556 . ?
O1 Ba2 Y1 90.0 . . ?
O1 Ba2 Y1 90.0 3 . ?
B1 Ba2 Y1 90.000(1) 1_455 . ?
B1 Ba2 Y1 90.000(1) 8_666 . ?
B1 Ba2 Y1 90.0 3_545 . ?
Y1 Ba2 Y1 180.0 2 . ?
O3 Ba2 Ba1 99.66(13) 1_455 1_445 ?
O3 Ba2 Ba1 31.91(8) 3_545 1_445 ?
O3 Ba2 Ba1 132.93(12) 8_666 1_445 ?
O1 Ba2 Ba1 55.54(12) 8_556 1_445 ?
O1 Ba2 Ba1 71.21(13) . 1_445 ?
O1 Ba2 Ba1 152.63(4) 3 1_445 ?
B1 Ba2 Ba1 78.51(17) 1_455 1_445 ?
B1 Ba2 Ba1 149.19(10) 8_666 1_445 ?
B1 Ba2 Ba1 48.72(16) 3_545 1_445 ?
Y1 Ba2 Ba1 115.957(8) 2 1_445 ?
Y1 Ba2 Ba1 64.043(8) . 1_445 ?
B1 O1 B1 124.3(10) . 3_545 ?
B1 O1 Ba2 145.7(6) . . ?
B1 O1 Ba2 90.0(6) 3_545 . ?
B2 O2 B2 123.3(7) 1_655 3 ?
B2 O2 Ba1 141.1(5) 1_655 . ?
B2 O2 Ba1 91.5(4) 3 . ?
B1 O3 Ba2 100.1(6) . 1_655 ?
B1 O3 Ba1 114.7(4) . 8_666 ?
Ba2 O3 Ba1 116.19(18) 1_655 8_666 ?
B1 O3 Ba1 114.7(4) . . ?
Ba2 O3 Ba1 116.19(18) 1_655 . ?
Ba1 O3 Ba1 96.0(2) 8_666 . ?
O3 B1 O1 124.2(9) . . ?
O3 B1 O1 120.1(9) . 8_656 ?
O1 B1 O1 115.7(10) . 8_656 ?
O3 B1 Ba2 56.3(5) . 1_655 ?
O1 B1 Ba2 179.5(7) . 1_655 ?
O1 B1 Ba2 63.8(5) 8_656 1_655 ?
O3 B1 Ba1 45.3(3) . 8_666 ?
O1 B1 Ba1 93.2(5) . 8_666 ?
O1 B1 Ba1 135.0(4) 8_656 8_666 ?
Ba2 B1 Ba1 87.2(2) 1_655 8_666 ?
O3 B1 Ba1 45.3(3) . . ?
O1 B1 Ba1 93.2(5) . . ?
O1 B1 Ba1 135.0(4) 8_656 . ?
Ba2 B1 Ba1 87.2(2) 1_655 . ?
Ba1 B1 Ba1 71.1(2) 8_666 . ?
B2 O4 Y1 121.7(4) . . ?
B2 O4 Ba1 97.8(4) . 1_445 ?
Y1 O4 Ba1 131.9(2) . 1_445 ?
O4 B2 O2 123.0(6) . 1_455 ?
O4 B2 O2 120.2(6) . 5 ?
O2 B2 O2 116.7(7) 1_455 5 ?
O4 B2 Ba1 59.2(4) . 1_445 ?
O2 B2 Ba1 166.8(5) 1_455 1_445 ?
O2 B2 Ba1 63.6(3) 5 1_445 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ba1 O3 2.715(5) 8_666 ?
Ba1 O3 2.715(5) . ?
Ba1 O3 2.715(5) 3_655 ?
Ba1 O4 2.889(5) 3 ?
Ba1 O4 2.889(5) 1_665 ?
Ba1 O4 2.889(5) 5_655 ?
Ba1 O2 2.988(5) 5_665 ?
Ba1 O2 2.988(5) 3_655 ?
Ba1 O2 2.988(5) . ?
Ba1 B2 3.334(7) 1_665 ?
Ba1 B2 3.334(7) 3 ?
Ba1 B2 3.334(7) 5_655 ?
Y1 O4 2.252(5) 9 ?
Y1 O4 2.252(5) 5 ?
Y1 O4 2.252(5) 11 ?
Y1 O4 2.252(5) 7 ?
Y1 O4 2.252(5) 3 ?
Y1 O4 2.253(5) . ?
Y1 Ba2 4.2414(5) 7 ?
Y1 Ba2 4.2414(5) . ?
Ba2 O3 2.714(7) 1_455 ?
Ba2 O3 2.714(7) 3_545 ?
Ba2 O3 2.714(7) 8_666 ?
Ba2 O1 2.880(7) 8_556 ?
Ba2 O1 2.880(7) . ?
Ba2 O1 2.880(7) 3 ?
Ba2 B1 3.211(11) 1_455 ?
Ba2 B1 3.211(11) 8_666 ?
Ba2 B1 3.211(11) 3_545 ?
Ba2 Y1 4.2414(5) 2 ?
Ba2 Ba1 4.6083(4) 1_445 ?
O1 B1 1.394(13) . ?
O1 B1 1.418(13) 3_545 ?
O2 B2 1.400(9) 1_655 ?
O2 B2 1.401(9) 3 ?
O3 B1 1.303(12) . ?
O3 Ba2 2.714(7) 1_655 ?
O3 Ba1 2.715(5) 8_666 ?
B1 O1 1.418(13) 8_656 ?
B1 Ba2 3.211(11) 1_655 ?
B1 Ba1 3.467(9) 8_666 ?
O4 B2 1.319(9) . ?
O4 Ba1 2.889(5) 1_445 ?
B2 O2 1.400(9) 1_455 ?
B2 O2 1.401(9) 5 ?
B2 Ba1 3.334(7) 1_445 ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O4 Y1 Ba2 O3 -10.3(2) 9 . . 1_455 ?
O4 Y1 Ba2 O3 49.7(2) 5 . . 1_455 ?
O4 Y1 Ba2 O3 -130.3(2) 11 . . 1_455 ?
O4 Y1 Ba2 O3 109.7(2) 7 . . 1_455 ?
O4 Y1 Ba2 O3 169.7(2) 3 . . 1_455 ?
O4 Y1 Ba2 O3 -70.3(2) . . . 1_455 ?
Ba2 Y1 Ba2 O3 169.25(15) 7 . . 1_455 ?
O4 Y1 Ba2 O3 109.7(2) 9 . . 3_545 ?
O4 Y1 Ba2 O3 169.7(2) 5 . . 3_545 ?
O4 Y1 Ba2 O3 -10.3(2) 11 . . 3_545 ?
O4 Y1 Ba2 O3 -130.3(2) 7 . . 3_545 ?
O4 Y1 Ba2 O3 -70.3(2) 3 . . 3_545 ?
O4 Y1 Ba2 O3 49.7(2) . . . 3_545 ?
Ba2 Y1 Ba2 O3 -70.75(15) 7 . . 3_545 ?
O4 Y1 Ba2 O3 -130.3(2) 9 . . 8_666 ?
O4 Y1 Ba2 O3 -70.3(2) 5 . . 8_666 ?
O4 Y1 Ba2 O3 109.7(2) 11 . . 8_666 ?
O4 Y1 Ba2 O3 -10.3(2) 7 . . 8_666 ?
O4 Y1 Ba2 O3 49.7(2) 3 . . 8_666 ?
O4 Y1 Ba2 O3 169.7(2) . . . 8_666 ?
Ba2 Y1 Ba2 O3 49.25(14) 7 . . 8_666 ?
O4 Y1 Ba2 O1 39.5(2) 9 . . 8_556 ?
O4 Y1 Ba2 O1 99.5(2) 5 . . 8_556 ?
O4 Y1 Ba2 O1 -80.5(2) 11 . . 8_556 ?
O4 Y1 Ba2 O1 159.5(2) 7 . . 8_556 ?
O4 Y1 Ba2 O1 -140.5(2) 3 . . 8_556 ?
O4 Y1 Ba2 O1 -20.5(2) . . . 8_556 ?
Ba2 Y1 Ba2 O1 -141.00(14) 7 . . 8_556 ?
O4 Y1 Ba2 O1 159.5(2) 9 . . . ?
O4 Y1 Ba2 O1 -140.5(2) 5 . . . ?
O4 Y1 Ba2 O1 39.5(2) 11 . . . ?
O4 Y1 Ba2 O1 -80.5(2) 7 . . . ?
O4 Y1 Ba2 O1 -20.5(2) 3 . . . ?
O4 Y1 Ba2 O1 99.5(2) . . . . ?
Ba2 Y1 Ba2 O1 -21.00(14) 7 . . . ?
O4 Y1 Ba2 O1 -80.5(2) 9 . . 3 ?
O4 Y1 Ba2 O1 -20.5(2) 5 . . 3 ?
O4 Y1 Ba2 O1 159.5(2) 11 . . 3 ?
O4 Y1 Ba2 O1 39.5(2) 7 . . 3 ?
O4 Y1 Ba2 O1 99.5(2) 3 . . 3 ?
O4 Y1 Ba2 O1 -140.5(2) . . . 3 ?
Ba2 Y1 Ba2 O1 99.00(14) 7 . . 3 ?
O4 Y1 Ba2 B1 13.3(3) 9 . . 1_455 ?
O4 Y1 Ba2 B1 73.3(3) 5 . . 1_455 ?
O4 Y1 Ba2 B1 -106.7(3) 11 . . 1_455 ?
O4 Y1 Ba2 B1 133.3(3) 7 . . 1_455 ?
O4 Y1 Ba2 B1 -166.7(3) 3 . . 1_455 ?
O4 Y1 Ba2 B1 -46.7(3) . . . 1_455 ?
Ba2 Y1 Ba2 B1 -167.20(19) 7 . . 1_455 ?
O4 Y1 Ba2 B1 -106.7(3) 9 . . 8_666 ?
O4 Y1 Ba2 B1 -46.7(3) 5 . . 8_666 ?
O4 Y1 Ba2 B1 133.3(3) 11 . . 8_666 ?
O4 Y1 Ba2 B1 13.3(3) 7 . . 8_666 ?
O4 Y1 Ba2 B1 73.3(3) 3 . . 8_666 ?
O4 Y1 Ba2 B1 -166.7(3) . . . 8_666 ?
Ba2 Y1 Ba2 B1 72.80(19) 7 . . 8_666 ?
O4 Y1 Ba2 B1 133.3(3) 9 . . 3_545 ?
O4 Y1 Ba2 B1 -166.7(3) 5 . . 3_545 ?
O4 Y1 Ba2 B1 13.3(3) 11 . . 3_545 ?
O4 Y1 Ba2 B1 -106.7(3) 7 . . 3_545 ?
O4 Y1 Ba2 B1 -46.7(3) 3 . . 3_545 ?
O4 Y1 Ba2 B1 73.3(3) . . . 3_545 ?
Ba2 Y1 Ba2 B1 -47.20(19) 7 . . 3_545 ?
O4 Y1 Ba2 Y1 -179.51(17) 9 . . 2 ?
O4 Y1 Ba2 Y1 -119.51(17) 5 . . 2 ?
O4 Y1 Ba2 Y1 60.49(17) 11 . . 2 ?
O4 Y1 Ba2 Y1 -59.51(17) 7 . . 2 ?
O4 Y1 Ba2 Y1 0.49(17) 3 . . 2 ?
O4 Y1 Ba2 Y1 120.49(17) . . . 2 ?
Ba2 Y1 Ba2 Y1 0.0 7 . . 2 ?
O4 Y1 Ba2 Ba1 90.49(17) 9 . . 1_445 ?
O4 Y1 Ba2 Ba1 150.49(17) 5 . . 1_445 ?
O4 Y1 Ba2 Ba1 -29.51(17) 11 . . 1_445 ?
O4 Y1 Ba2 Ba1 -149.51(17) 7 . . 1_445 ?
O4 Y1 Ba2 Ba1 -89.51(17) 3 . . 1_445 ?
O4 Y1 Ba2 Ba1 30.49(17) . . . 1_445 ?
Ba2 Y1 Ba2 Ba1 -90.0 7 . . 1_445 ?
O3 Ba2 O1 B1 180.0 1_455 . . . ?
O3 Ba2 O1 B1 180.0 3_545 . . . ?
O3 Ba2 O1 B1 0.0 8_666 . . . ?
O1 Ba2 O1 B1 180.0 8_556 . . . ?
O1 Ba2 O1 B1 0.0 3 . . . ?
B1 Ba2 O1 B1 180.0 1_455 . . . ?
B1 Ba2 O1 B1 0.0 8_666 . . . ?
B1 Ba2 O1 B1 180.0 3_545 . . . ?
Y1 Ba2 O1 B1 -90.000(1) 2 . . . ?
Y1 Ba2 O1 B1 90.0 . . . . ?
Ba1 Ba2 O1 B1 152.46(2) 1_445 . . . ?
O3 Ba2 O1 B1 0.0 1_455 . . 3_545 ?
O3 Ba2 O1 B1 0.0 3_545 . . 3_545 ?
O3 Ba2 O1 B1 180.0 8_666 . . 3_545 ?
O1 Ba2 O1 B1 0.0 8_556 . . 3_545 ?
O1 Ba2 O1 B1 180.0 3 . . 3_545 ?
B1 Ba2 O1 B1 0.0 1_455 . . 3_545 ?
B1 Ba2 O1 B1 180.0 8_666 . . 3_545 ?
Y1 Ba2 O1 B1 90.0 2 . . 3_545 ?
Y1 Ba2 O1 B1 -90.000(1) . . . 3_545 ?
Ba1 Ba2 O1 B1 -27.54(2) 1_445 . . 3_545 ?
O3 Ba1 O2 B2 -110.6(7) 8_666 . . 1_655 ?
O3 Ba1 O2 B2 -50.8(7) . . . 1_655 ?
O3 Ba1 O2 B2 -30.4(8) 3_655 . . 1_655 ?
O4 Ba1 O2 B2 -164.5(8) 3 . . 1_655 ?
O4 Ba1 O2 B2 131.2(7) 1_665 . . 1_655 ?
O4 Ba1 O2 B2 35.2(7) 5_655 . . 1_655 ?
O2 Ba1 O2 B2 177.3(6) 5_665 . . 1_655 ?
O2 Ba1 O2 B2 49.6(9) 3_655 . . 1_655 ?
B2 Ba1 O2 B2 163.1(8) 1_665 . . 1_655 ?
B2 Ba1 O2 B2 -155.0(11) 3 . . 1_655 ?
B2 Ba1 O2 B2 38.3(7) 5_655 . . 1_655 ?
O3 Ba1 O2 B2 44.4(5) 8_666 . . 3 ?
O3 Ba1 O2 B2 104.2(5) . . . 3 ?
O3 Ba1 O2 B2 124.6(4) 3_655 . . 3 ?
O4 Ba1 O2 B2 -9.5(4) 3 . . 3 ?
O4 Ba1 O2 B2 -73.8(5) 1_665 . . 3 ?
O4 Ba1 O2 B2 -169.9(5) 5_655 . . 3 ?
O2 Ba1 O2 B2 -27.8(5) 5_665 . . 3 ?
O2 Ba1 O2 B2 -155.4(3) 3_655 . . 3 ?
B2 Ba1 O2 B2 -41.9(4) 1_665 . . 3 ?
B2 Ba1 O2 B2 -166.7(5) 5_655 . . 3 ?
O3 Ba1 O3 B1 82.8(6) 8_666 . . . ?
O3 Ba1 O3 B1 158.5(6) 3_655 . . . ?
O4 Ba1 O3 B1 5.9(6) 3 . . . ?
O4 Ba1 O3 B1 141.4(5) 1_665 . . . ?
O4 Ba1 O3 B1 -106.5(5) 5_655 . . . ?
O2 Ba1 O3 B1 62.9(6) 5_665 . . . ?
O2 Ba1 O3 B1 -143.9(5) 3_655 . . . ?
O2 Ba1 O3 B1 -36.4(5) . . . . ?
B2 Ba1 O3 B1 99.7(6) 1_665 . . . ?
B2 Ba1 O3 B1 -11.5(5) 3 . . . ?
B2 Ba1 O3 B1 -126.8(6) 5_655 . . . ?
O3 Ba1 O3 Ba2 -160.9(3) 8_666 . . 1_655 ?
O3 Ba1 O3 Ba2 -85.2(4) 3_655 . . 1_655 ?
O4 Ba1 O3 Ba2 122.1(2) 3 . . 1_655 ?
O4 Ba1 O3 Ba2 -102.3(3) 1_665 . . 1_655 ?
O4 Ba1 O3 Ba2 9.77(19) 5_655 . . 1_655 ?
O2 Ba1 O3 Ba2 179.09(16) 5_665 . . 1_655 ?
O2 Ba1 O3 Ba2 -27.6(3) 3_655 . . 1_655 ?
O2 Ba1 O3 Ba2 79.8(2) . . . 1_655 ?
B2 Ba1 O3 Ba2 -144.1(3) 1_665 . . 1_655 ?
B2 Ba1 O3 Ba2 104.7(2) 3 . . 1_655 ?
B2 Ba1 O3 Ba2 -10.5(2) 5_655 . . 1_655 ?
O3 Ba1 O3 Ba1 -37.85(5) 8_666 . . 8_666 ?
O3 Ba1 O3 Ba1 37.85(5) 3_655 . . 8_666 ?
O4 Ba1 O3 Ba1 -114.8(2) 3 . . 8_666 ?
O4 Ba1 O3 Ba1 20.8(4) 1_665 . . 8_666 ?
O4 Ba1 O3 Ba1 132.9(2) 5_655 . . 8_666 ?
O2 Ba1 O3 Ba1 -57.8(3) 5_665 . . 8_666 ?
O2 Ba1 O3 Ba1 95.5(2) 3_655 . . 8_666 ?
O2 Ba1 O3 Ba1 -157.1(2) . . . 8_666 ?
B2 Ba1 O3 Ba1 -21.0(4) 1_665 . . 8_666 ?
B2 Ba1 O3 Ba1 -132.2(2) 3 . . 8_666 ?
B2 Ba1 O3 Ba1 112.6(2) 5_655 . . 8_666 ?
Ba2 O3 B1 O1 180.0 1_655 . . . ?
Ba1 O3 B1 O1 54.9(3) 8_666 . . . ?
Ba1 O3 B1 O1 -54.9(3) . . . . ?
Ba2 O3 B1 O1 0.0 1_655 . . 8_656 ?
Ba1 O3 B1 O1 -125.1(3) 8_666 . . 8_656 ?
Ba1 O3 B1 O1 125.1(3) . . . 8_656 ?
Ba1 O3 B1 Ba2 -125.1(3) 8_666 . . 1_655 ?
Ba1 O3 B1 Ba2 125.1(3) . . . 1_655 ?
Ba2 O3 B1 Ba1 125.1(3) 1_655 . . 8_666 ?
Ba1 O3 B1 Ba1 -109.7(6) . . . 8_666 ?
Ba2 O3 B1 Ba1 -125.1(3) 1_655 . . . ?
Ba1 O3 B1 Ba1 109.7(6) 8_666 . . . ?
B1 O1 B1 O3 180.0 3_545 . . . ?
Ba2 O1 B1 O3 0.0 . . . . ?
B1 O1 B1 O1 0.0 3_545 . . 8_656 ?
Ba2 O1 B1 O1 180.0 . . . 8_656 ?
B1 O1 B1 Ba2 0.0 3_545 . . 1_655 ?
Ba2 O1 B1 Ba2 180.0 . . . 1_655 ?
B1 O1 B1 Ba1 -144.36(12) 3_545 . . 8_666 ?
Ba2 O1 B1 Ba1 35.64(12) . . . 8_666 ?
B1 O1 B1 Ba1 144.36(12) 3_545 . . . ?
Ba2 O1 B1 Ba1 -35.64(12) . . . . ?
O3 Ba1 B1 O3 -89.9(6) 8_666 . . . ?
O3 Ba1 B1 O3 -20.2(6) 3_655 . . . ?
O4 Ba1 B1 O3 -173.8(6) 3 . . . ?
O4 Ba1 B1 O3 -72.2(9) 1_665 . . . ?
O4 Ba1 B1 O3 70.5(5) 5_655 . . . ?
O2 Ba1 B1 O3 -131.2(5) 5_665 . . . ?
O2 Ba1 B1 O3 42.1(6) 3_655 . . . ?
O2 Ba1 B1 O3 136.0(6) . . . . ?
B2 Ba1 B1 O3 -108.3(6) 1_665 . . . ?
B2 Ba1 B1 O3 166.5(6) 3 . . . ?
B2 Ba1 B1 O3 54.7(6) 5_655 . . . ?
O3 Ba1 B1 O1 47.4(3) 8_666 . . . ?
O3 Ba1 B1 O1 137.4(7) . . . . ?
O3 Ba1 B1 O1 117.1(3) 3_655 . . . ?
O4 Ba1 B1 O1 -36.4(3) 3 . . . ?
O4 Ba1 B1 O1 65.1(7) 1_665 . . . ?
O4 Ba1 B1 O1 -152.1(4) 5_655 . . . ?
O2 Ba1 B1 O1 6.1(4) 5_665 . . . ?
O2 Ba1 B1 O1 179.5(3) 3_655 . . . ?
O2 Ba1 B1 O1 -86.7(4) . . . . ?
B2 Ba1 B1 O1 29.1(5) 1_665 . . . ?
B2 Ba1 B1 O1 -56.2(4) 3 . . . ?
B2 Ba1 B1 O1 -168.0(3) 5_655 . . . ?
O3 Ba1 B1 O1 179.6(8) 8_666 . . 8_656 ?
O3 Ba1 B1 O1 -90.5(11) . . . 8_656 ?
O3 Ba1 B1 O1 -110.8(8) 3_655 . . 8_656 ?
O4 Ba1 B1 O1 95.7(8) 3 . . 8_656 ?
O4 Ba1 B1 O1 -162.8(5) 1_665 . . 8_656 ?
O4 Ba1 B1 O1 -20.0(8) 5_655 . . 8_656 ?
O2 Ba1 B1 O1 138.3(7) 5_665 . . 8_656 ?
O2 Ba1 B1 O1 -48.4(8) 3_655 . . 8_656 ?
O2 Ba1 B1 O1 45.4(7) . . . 8_656 ?
B2 Ba1 B1 O1 161.2(7) 1_665 . . 8_656 ?
B2 Ba1 B1 O1 76.0(7) 3 . . 8_656 ?
B2 Ba1 B1 O1 -35.8(8) 5_655 . . 8_656 ?
O3 Ba1 B1 Ba2 -132.86(19) 8_666 . . 1_655 ?
O3 Ba1 B1 Ba2 -42.9(5) . . . 1_655 ?
O3 Ba1 B1 Ba2 -63.17(18) 3_655 . . 1_655 ?
O4 Ba1 B1 Ba2 143.27(18) 3 . . 1_655 ?
O4 Ba1 B1 Ba2 -115.2(5) 1_665 . . 1_655 ?
O4 Ba1 B1 Ba2 27.58(14) 5_655 . . 1_655 ?
O2 Ba1 B1 Ba2 -174.16(14) 5_665 . . 1_655 ?
O2 Ba1 B1 Ba2 -0.8(2) 3_655 . . 1_655 ?
O2 Ba1 B1 Ba2 93.0(2) . . . 1_655 ?
B2 Ba1 B1 Ba2 -151.2(3) 1_665 . . 1_655 ?
B2 Ba1 B1 Ba2 123.5(2) 3 . . 1_655 ?
B2 Ba1 B1 Ba2 11.75(18) 5_655 . . 1_655 ?
O3 Ba1 B1 Ba1 -44.88(16) 8_666 . . 8_666 ?
O3 Ba1 B1 Ba1 45.0(5) . . . 8_666 ?
O3 Ba1 B1 Ba1 24.81(18) 3_655 . . 8_666 ?
O4 Ba1 B1 Ba1 -128.8(2) 3 . . 8_666 ?
O4 Ba1 B1 Ba1 -27.2(6) 1_665 . . 8_666 ?
O4 Ba1 B1 Ba1 115.56(17) 5_655 . . 8_666 ?
O2 Ba1 B1 Ba1 -86.2(2) 5_665 . . 8_666 ?
O2 Ba1 B1 Ba1 87.2(2) 3_655 . . 8_666 ?
O2 Ba1 B1 Ba1 -179.0(3) . . . 8_666 ?
B2 Ba1 B1 Ba1 -63.2(4) 1_665 . . 8_666 ?
B2 Ba1 B1 Ba1 -148.5(3) 3 . . 8_666 ?
B2 Ba1 B1 Ba1 99.74(18) 5_655 . . 8_666 ?
O4 Y1 O4 B2 -19.1(5) 9 . . . ?
O4 Y1 O4 B2 74.6(7) 5 . . . ?
O4 Y1 O4 B2 -105.4(7) 11 . . . ?
O4 Y1 O4 B2 155(3) 7 . . . ?
O4 Y1 O4 B2 160.9(5) 3 . . . ?
Ba2 Y1 O4 B2 -62.3(6) 7 . . . ?
Ba2 Y1 O4 B2 117.7(6) . . . . ?
O4 Y1 O4 Ba1 121.2(4) 9 . . 1_445 ?
O4 Y1 O4 Ba1 -145.1(2) 5 . . 1_445 ?
O4 Y1 O4 Ba1 34.9(2) 11 . . 1_445 ?
O4 Y1 O4 Ba1 -65(3) 7 . . 1_445 ?
O4 Y1 O4 Ba1 -58.8(4) 3 . . 1_445 ?
Ba2 Y1 O4 Ba1 78.0(3) 7 . . 1_445 ?
Ba2 Y1 O4 Ba1 -102.0(3) . . . 1_445 ?
Y1 O4 B2 O2 -44.0(10) . . . 1_455 ?
Ba1 O4 B2 O2 164.6(6) 1_445 . . 1_455 ?
Y1 O4 B2 O2 132.6(6) . . . 5 ?
Ba1 O4 B2 O2 -18.8(7) 1_445 . . 5 ?
Y1 O4 B2 Ba1 151.3(5) . . . 1_445 ?
